Table 35. Continued. 



Alloy 



Stress 

 (ksi) 



Percent 



Yield 



Strength 



Exposure 



(day) 



Depth 

 (ft) 



Number of 



Specimens 



Exposed 



Number 

 Failed 



Source 1 * 



Ni-Be, 1/2 H 

 Ni-Be, 1/2 H 

 Ni-Be, 1/2 H 



Ni-Be, 1/2 HT 

 Ni-Be, 1/2 HT 

 Ni-Be, 1/2 HT 



93 

 37 

 93 



60 

 60 

 60 



75 

 30 



75 



30 

 30 

 30 



197 

 402 

 402 



403 

 197 

 402 



2,340 

 2,370 

 2,370 



6,780 

 2,340* 



2,370 



3 

 3 

 3 



3 

 3 

 3 





 

 





 

 



NADC (7) 

 NADC (7) 

 NADC (7) 



NADC (7) 

 NADC (7) 

 NADC (7) 



a Numbers refer to references at end of report. 



'Severe corrosion at sheared edges indicating possible susceptibility to stress corrosion cracking. 



127 



